advertisement

PHYSICAL REVIEW B 66, 012512 共2002兲 Generalized method of image and the tunneling spectroscopy in high-T c superconductors Shin-Tza Wu1 and Chung-Yu Mou1,2 1 Department of Physics, National Tsing Hua University, Hsinchu 30043, Taiwan 2 National Center for Theoretical Sciences, P.O. Box 2-131, Hsinchu, Taiwan 共Received 7 May 2002; published 10 July 2002兲 A generalized method of image is developed to investigate the tunneling spectrum from the metal into a class of states, with the tight-binding dispersion fully included. The broken reflection symmetry is shown to be the necessary condition for the appearance of the zero-bias conductance peak 共ZBCP兲. Applying this method to the d-wave superconductor yields results in agreement with experiments regarding the splitting of ZBCP’s in magnetic fields. Furthermore, a ZBCP is predicted for tunneling into the 共110兲 direction of the d-density-wave state, providing a signature to look for in experiments. DOI: 10.1103/PhysRevB.66.012512 PACS number共s兲: 74.20.Mn, 74.50.⫹r, 74.80.Fp The current transport through a heterojunction consisting of a normal metal and another different material 共X兲 has been a subject of interest for many years. In this setup, the normal metal with known spectral properties is used as a probe to analyze the electronic states of the material X.1 Although such measurements have provided useful insights into the bulk spectral properties of X, it has been also realized that the presence of the interface matters. The zero-bias conductance peak 共ZBCP兲 observed in the tunneling spectra when X is a d-wave superconductor 共ND junction兲 in the 共110兲 direction2 is a well-known example of interface effects. However, the issue of exactly how the tunneling measurements are related to the bulk properties has never been answered satisfactorily. Conventionally, the ND junction is analyzed in the meanfield level, using the Bogoliubov–de Gennes 共BdG兲 equations in which continuum and quasiclassical approximations are often invoked. While these approximations are valid for conventional superconductors, they are certainly not justified for high-T c cuprates where proximity to the Mott insulators entails fully consideration of the tight-binding nature. Previously,3 this was done by numerically solving the discrete BdG equation for each interface orientation individually without elucidating their relations to the bulk properties. This technical inconvenience makes it difficult to include fluctuations systematically in this approach. In this work, we shall adopt a different approach based on the nonequilibrium Keldysh-Green’s function formalism which enables one to construct systematically higher-order corrections from the mean-field lattice Green’s functions.4 – 6 In this approach, because X extends over a semi-infinite space, one shall need the half-space Green’s functions. For simple configurations such as the 共100兲 orientation of a d-wave superconductor, it turns out that these half-space Green’s functions only differ from the bulk ones by sinusoidal factors. This relation certainly does not hold for other orientations as it predicts no ZBCP in the 共110兲 direction. We shall develop a generalized method of image which enables us to construct half-space Green’s functions from the bulk ones. We emphasize the generality of this method and its ability to account for the low-energy features in the tunneling spectrum for a whole class of states. As a demonstration, in this paper we will focus mostly on the study of ND junctions 0163-1829/2002/66共1兲/012512共4兲/$20.00 and only briefly mention the applications to other systems. The effects of interactions and fluctuations will be addressed elsewhere. Our results indicate broken reflection symmetry is necessary for the emergence of ZBCP’s. For ND junctions our method can reproduce earlier results on the ZBCP in the continuous-wave approximation.2,7 In a full tight-binding calculation for 共110兲 and 共210兲 directions, we obtain the doping dependence of ZBCP’s which exhibits its sensitivity to the Fermi surface topology. In particular, the splitting of the ZBCP in the current-carrying state is also calculated and is shown to be in agreement with experiments. At the end, we analyze the case when X is the d-density-wave 共DDW兲 state in 共110兲 direction and the semi-infinite graphene sheet with a zigzag-type interface. The former state was recently proposed as a possible normal state for high-T c cuprates.8 Conductance peaks are found for both states. We start by considering a junction consisting of a twodimensional 共2D兲 normal metal on the left 共L兲 hand side (⫺⬁⬍x⭐⫺d, where d is the lattice constant of the metal side兲 and a d-wave superconductor (0⭐x⬍⬁) on the right 共R兲 hand side 共see Fig. 1兲, governed by the Hamiltonians H L and H R , respectively. At the mean-field level, we have H R ⫽⫺ ⫹ 兺 具i j典, t R c i† c j ⫺ t R⬘ c i† c j 兺 i j , 具 典⬘ ⌬ i j 共 c i↑ c j↓ ⫺c i↓ c j↑ 兲 ⫹H.c., 兺 具i j典 共1兲 where 具 i j 典 denotes the nearest-neighbor 共NN兲 bond, 具 i j 典 ⬘ the next-NN bond, and ⌬ i j possesses d-wave symmetry. The tunneling Hamiltonian connects the interface points at x ⫽⫺d and x⫽0, and is given by H T ⫽ 兺 y t( 兩 y L ⫺y R 兩 )(c L† c R ⫹c R† c L ), where the summation is over lattice points along the interface, chosen to be in the y direction. We shall assume that both sides are square lattices and characterize the orientation of right-hand side 共RHS兲 by the Miller indices (hk0). The total grand Hamiltonian is then given by K⫽(H L ⫺ L N L )⫹(H R ⫺ R N R )⫹H T ⬅K 0 ⫹H T . Here L and R are the chemical potentials and their difference L ⫺ R is fixed to be the voltage drop eV across the junction. 66 012512-1 ©2002 The American Physical Society PHYSICAL REVIEW B 66, 012512 共2002兲 BRIEF REPORTS t R⬘ ⫽0. In this case, we are looking for the Green’s function Ḡ 0 ( ,k y, x,x ⬘ ) 共which is a 2⫻2 matrix in Nambu’s notation兲, which satisfies the boundary condition Ḡ 0 ⫽0 at x ⫽⫺d/2. We shall suppress the dependence on and k y . Here, since x ⬘ is the location of the point source and its image point is at ⫺d⫺x ⬘ ,9 the method of image can be employed by constructing Ḡ 0 共 x,x ⬘ 兲 ⫽G 0 共 x⫺x ⬘ 兲 ⫺G 0 共 x⫹d⫹x ⬘ 兲 ␣ 共 x ⬘ 兲 , FIG. 1. Schematic plot of the ND junction in the 共110兲 and 共210兲 directions. Here two hard walls for the 共210兲 case are at A ⫽⫺2d/ 冑5 and B⫽⫺2d/ 冑5. The dots on the x axis are the reduced 1D lattice points. In the nonequilibrium Keldysh-Green’s function formalism, H T is adiabatically turned on.4,5 As a result, the bare Green’s function is defined only on a half-plane. Since the nearest-neighboring bonds to the interface sites are cut, there is effectively a hard wall located at say, for the 共110兲 interface, x⫽⫺d/2. This hard-wall boundary condition prompts the application of the method of image. However, because lattice points in the half-plane usually do not form a simple Bravais lattice and the d-wave gap changes sign under reflection, the implementation of the conventional method of image appears problematic. To overcome these difficulties, a Fourier transform in the y direction is performed first. Consider the case of 共110兲 orientations; the Hamiltonian with only NN hopping becomes H R⫽ 兺 i, ,k ⫹ 冉 冊 冉 冊 ⫺2t R cos y 2i⌬ 0 sin 兺 i,k y k yd † c i 共 k y 兲 c i⫹1 共 k y 兲 2 k yd 关 c i↑ 共 k y 兲 c i⫹1↓ 共 ⫺k y 兲 2 ⫹c i↓ 共 ⫺k y 兲 c i⫹1↑ 共 k y 兲兴 ⫹H.c., 共2兲 where ⫺ /d⬍k y ⭐ /d and 2⌬ 0 is the gap value. The whole problem is now one dimensional, and the hard wall becomes a point. Note that the suppression of the gap near the interface can be taken into account by adding selfconsistent ␦ ⌬ 0 (i) to Eq.共2兲 and can be treated perturbatively later. In the presence of t R⬘ , additional terms 兺 i, ,k y ⫺2t R⬘ cos(kyd)ci†(ky)ci(ky)⫹tR⬘ ci†(ky)ci⫹2(ky)⫹H.c. appear. Since at the boundary, both t R and t R⬘ are cut and become dangling bonds, one needs to introduce two hard walls at x ⫽⫺d/2 and x⫽⫺d. For clear presentation, we shall first set 共3兲 where G 0 is the bulk bare Green’s function and ␣ is a matrix to be determined. The first term is the direct propagation from x ⬘ to x, while the second term will reduce to the propagation from the image point to x in special situations 共see below兲. In fact, since Ḡ 0 has to vanish at x⫽⫺d/2, we obtain ␣ (x ⬘ )⫽G ⫺1 0 (d/2⫹x ⬘ )G 0 (⫺d/2⫺x ⬘ ). Therefore, the second term describes the propagation from x ⬘ to x via the reflection of the hard wall. The matrix ␣ , apart from fitting the boundary condition, carries important information about the gap structure along the reflected path from x ⬘ to x. Note that in calculating the tunneling current, since H T only connects points along the interface, only the surface Green’s function ḡ 0 ( ,k y )⬅Ḡ 0 (x⫽0,x ⬘ ⫽0) is needed.4,10 Writing G 0 in the Fourier k x space, we find ḡ 0 共 ,k y 兲 ⬅ 冕 2 /d dk x G 0 共 ,k y, k x 兲关 1⫺exp共 ik x d 兲 ␣ 0 兴 , ⫺2 /d 2 ␣ 0 ⫽G ⫺1 0 (d/2)G 0 (⫺d/2) 共4兲 is independent of where the factor k x . If the reflection symmetry holds for the state X, such as d-wave superconductors in 共100兲 direction 共in this case, d/2 is replaced by d), one has ␣ 0 ⫽1 and hence it reduces to the 2 /d ḡ 0 ( ,k y )⬅ 兰 ⫺2 familiar form4 /d dk x / G 0 ( ,k y, k x ) 2 sin (kxd/2). Therefore, apart from modifications due to the sinusoidal factors, the density of state almost has the same feature as the bulk one. However, for other orientations such as the 共110兲 direction, reflection symmetry with respect to the interface is broken. As a result, ␣ 0 is not the identity matrix and as we shall see, this will give rise to the ZBCP. The advantage of Eq. 共4兲 is that it is purely based on the bulk Green’s functions. The interface orientation is encoded in k x and k y . In other words, G 0 ( ,k y ,k x ), which appears in Eq. 共4兲 and ␣ 0 is simply the usual bulk BCS Green’s function but with k being rotated by 45°. This technical merit is retained for other interface orientations but with k being rotated by an angle in accordance with the interface orientation. More importantly, this also offers a scheme for studying fluctuations and interactions. Essentially one can take into account these effects through the bulk Green’s function G 0 . This will be explained in more detail in a separate publication. When evaluating G 0 (x⫺x ⬘ ), the dominant contributions come from the poles determined by ( ⫹i ) 2 ⫺E 2k ⫽0, where E k ⫽ 冑⑀ 2k ⫹⌬ 2k . In the continuum limit, the dispersion 2 )/2m and ⌬ k ⫽⌬ 0 cos 2(⫺0), becomes ⑀ k ⫽ប 2 (k 2x ⫺k Fx 2 2 2 where k Fx ⫽k F ⫺k y , ⫽sin⫺1(ky /kF), and 0 is the angle between the crystal a axis and x direction. At the same 012512-2 PHYSICAL REVIEW B 66, 012512 共2002兲 BRIEF REPORTS FIG. 2. The total differential conductance of several dopings for the 共110兲 interface with ⫽0.01 and t L ⫽1.0. The weak link is modeled by the interface hopping t( )⫽exp关⫺冑( 0 ⫺ 兩 兩 )/⌫ 兴 with 0 ⫽11⌬ 0 and ⌫⫽⌬ 0 . Inset: dI/dV curve for the 共210兲 interface with ␦ ⫽0.08. time, the integration range of k x is extended to ⫾⬁. There are four poles located at ⫾k ⫾ with k ⫾ 冑 2 ⬅ k Fx ⫾2m 冑( ⫹i ) 2 ⫺ 兩 ⌬ ⫾ 兩 2 /ប 2 , representing particles and holes along different directions. Here ⌬ ⫾ are gaps in directions ⫾ . By contour integration, one obtains G 0 (x ⫺x ⬘ ) and thus ␣ (x ⬘ ). After some algebra and assuming that k F is large,11 indeed Eq. 共3兲 reproduces results obtained in Ref. 7 by directly solving the equations of motion. In our approach, the continuum approximation is not necessary. To investigate any effect that is due to the tight-binding nature, the full tight-binding dispersion has to be retained. In this case, the integration over k x cannot be extended to ⫾⬁, and thus poles are in different structure and a substantial difference from the continuum approximation could result. We now include the hopping t R⬘ for the 共110兲 direction. The main complication is to add a second hard wall at x ⫽⫺d. This is a simple generalization of the single hard-wall problem. One simply requires Ḡ 0 to vanish on all these hard walls simultaneously. Therefore, we write Ḡ 0 共 x,x ⬘ 兲 ⫽G 0 共 x⫺x ⬘ 兲 ⫺G 0 共 x⫺x 1⬘ 兲 ␣ 1 共 x ⬘ 兲 ⫺G 0 共 x⫺x 2⬘ 兲 ␣ 2 共 x ⬘ 兲 , 共5兲 where x ⬘1 ⫽⫺x ⬘ ⫺d and x ⬘2 ⫽⫺x ⬘ ⫺2d are images of x ⬘ . The boundary conditions at x⫽⫺d and x⫽⫺2d determine ␣ 1 and ␣ 2 . The surface Green’s function thus obtained is the bare one and will get renormalized by H T , giving rise to four different components in the differential conductance.4,11 The strength of H T , characterized by t, determines the relative weight among each component. In Fig. 2, we show our results for the spectrum of the total differential conductance for various dopings based on Eq. 共4兲. The parameters adopted are determined self-consistently from the mean-field slaveboson theory for the t-t ⬘ -J model.4 It is clear that the ZBCP’s are the most important features at low energies.2 Since the FIG. 3. The field dependence of the splitting for an underdoped case ( ␦ ⫽0.12). Inset: doping dependence of the splitting for a fixed magnetic field. ZBCP arises from the existence of zero-energy states, it must appear as poles at zero energy in the Green’s function. For the 共110兲 direction without t R⬘ , this is entirely determined by zeros of the denominator in ␣ :  共 ,k y 兲 ⫽det关 G 0 共 d/2兲兴 . 共6兲 In the continuum limit (d→0),  can be evaluated analyti¯ 2 ⫹(⌬ ⫹ / 兩 ⌬ ⫹ 兩 ⫹⌬ ⫺ / 兩 ⌬ ⫺ 兩 ) 2 兴 with ⌬ ¯ cally:  ⬇⫺ 关 2 /⌬ ⫽ 兩 ⌬ ⫹ 兩兩 ⌬ ⫺ 兩 /( 兩 ⌬ ⫹ 兩 ⫹ 兩 ⌬ ⫺ 兩 ). Therefore, poles of ḡ 0 at ⫽0 depend crucially on whether there is a sign change of the gap on the Fermi surface. This criterion, however, does not hold as one goes to the tight-binding limit because pairing no longer only occurs on the Fermi surface. As a result, a numerical computation of  is necessary. Our results indicate that ZBCP’s are sensitive to the Fermi surface topology. In fact, for the 共110兲 surface, the height of the peak depends on the volume of the Fermi surface. It reaches a maximum when R ⫽0 and decreases when R ⫽0. For other orientations, the ZBCP’s could even disappear. For general orientations, there could be more than one hard wall. As a demonstration, we consider the (210) interface. In this case, when t R⬘ ⫽0, two hard walls are located at x⫽⫺d/ 冑5 and ⫺2d/ 冑5, in analogy to the 共110兲 surface with t R⬘ . A typical result for the small scale of t is shown in the inset of Fig. 2. As t increases, the zero-energy states are able to leak out, and thus the ZBCP’s get broadened. Note that lattice points with dangling bonds form a pair-breaking region near the interface, resulting in the peaks around 2⌬ 0 . They are due to quasiparticle bound states with nonzero energy.12 The ZBCP’s split in the presence of magnetic fields H, essentially due to the Doppler shift caused by the supercurrent near the interface.13 In the tight-binding model, ⌬ i j is shifted to ⌬ i j exp关iq•(ri ⫹r j ) 兴 , where q⫽eH/2បc with being the penetration depth. By redefining c i ⫽c i exp(iq •ri ), the dependence on q can be absorbed into ⑀ k . Figure 3 shows the field dependence of the splitting for the 共110兲 in- 012512-3 PHYSICAL REVIEW B 66, 012512 共2002兲 BRIEF REPORTS FIG. 4. A typical dI/dV curve for tunneling into the 共110兲 direction of a d-density-wave state. Here R ⫽0 and ⌬ 0 ⫽0.1. Inset: a similar plot for tunneling from a wideband metal into the graphene sheet with zigzag interface. Here the hopping amplitude ␥ 0 ⫽0.1. terface, in agreement to recent experimental data.14 It is seen that for large H, the splitting deviates from linear dependence on H due to the lattice effect in our approach. The inset shows the doping dependence of splitting, reflecting its sensitive dependence on the Fermi surface topology. In fact, in the special case when particle-hole symmetry holds 共for example, R ⫽0 and t R⬘ ⫽0), we find that no matter how large E.L. Wolf, Principles of Electron Tunneling Spectroscopy 共Oxford University Press, New York, 1985兲. 2 C.R. Hu, Phys. Rev. Lett. 72, 1526 共1994兲; Y. Tanaka and S. Kashiwaya, ibid. 74, 3451 共1995兲. 3 See, for example, Y. Tamura, Y. Tanaka, M. Ogata, and S. Kashiwaya, Phys. Rev. B 60, 9817 共1999兲. 4 C.L. Wu et al., Phys. Rev. B 63, 172503 共2001兲; X.Z. Yan et al., ibid. 61, 14 759 共2000兲. 5 C. Caroli et al., J. Phys. C 4, 916 共1971兲; J.C. Cuevas et al., Phys. Rev. B 54, 7366 共1996兲. 6 The Green’s function approach has also been attempted at the quasiclassical level. See, for example, T. Luck et al., Phys. Rev. B 63, 064510 共2001兲. 1 H is, the ZBCP does not split at all, in consistent with naive expectations.11 Finally, our approach is easily modified to deal with other states. When X is the DDW, the two-component indices are associated with the two sublattices in this state. The formulation presented for the ND case can then be applied with minor modification.11 At 共110兲 orientation, the DDW state does not possess reflection symmetry; one thus expects ZBCP’s in this case. Figure 4 shows a typical result for tunneling into a DDW state in the 共110兲 direction when R ⫽0. Invariably, the ZBCP is present, consistent with a recent report.15 For finite R , unlike the d-wave superconductor, one simply adds R to the quasiparticle energy E k , 8 resulting in a shifting of the ZBCP to the bias at R . The existence of this conductance peak thus provides a signature of the DDW state. A similar analysis can be done for the semiinfinite graphene sheet. When projected onto 1D lattices it is then obvious that reflection symmetry is preserved in the case of the armchair interface while not in the zigzag case. This results in for the latter a ZBCP in the dI/dV curve 共see the inset of Fig. 4兲 共Ref. 11兲—consistent with previous numerical work.16 These two typical examples simply show that how easily our formulation can tell whether there should be ZBCP’s or not. Further applications to other systems will be reported elsewhere. It is our pleasure to thank Professor Sungkit Yip, Professor Hsiu-Hau Lin, and Professor T. K. Lee for useful discussions. This research was supported by NSC of Taiwan. M.P. Samanta and S. Datta, Phys. Rev. B 57, 10 972 共1998兲. S. Chakravarty et al., Phys. Rev. B 63, 094503 共2001兲. 9 In fact, for 1D, the image point can be chosen arbitrarily without affecting the result. 10 S. Datta, Electronic Transport in Mesoscopic Systems 共Cambridge University Press, New York, 1995兲. 11 S.T. Wu and C.-Y. Mou 共unpublished兲. 12 Y.S. Barush, A.A. Svidzinsky, and H. Burkhardt, Phys. Rev. B 55, 15 282 共1997兲. 13 M. Fogelstrom et al., Phys. Rev. Lett. 79, 281 共1997兲. 14 Y. Dagan and G. Deutscher, Phys. Rev. Lett. 87, 177004 共2001兲. 15 C. Honerkamp and M. Sigrist, cond-mat/0107550 共unpublished兲. 16 M. Fujita et al., J. Phys. Soc. Jpn. 65, 1920 共1996兲. 7 8 012512-4